**Abstract**

In this work, an attempt is made to characterize the electrical conductivity of ultra-thin films of tungsten(W). This is done by measuring on wafers that have films of W with a thickness between 0.57 and 8.5nm.

A method for characterizing ultra-thin films is by measuring their I-V relationship on circular transfer length method structures. This can give information about the film’s resistivity, contact resistance and transfer length. By looking at how non-linear the I-V relationship is, information can be obtained regarding the thickness at which the film goes from discontinuous to continuous. By measuring at various tempera-tures, the temperature coefficient of resistance (TCR) can be obtained.

It was found that the W layers on the tested wafers are highly non-homogeneous. As such, any characterizations from these tests are tentative. Nevertheless, some conclusions could still be drawn.

The thickness at which W films transition from semi-continuous to continuous is around 1.6nm. W films with a thickness up to at least 0.9nm have a highly non-linear I-V relationship, a negative TCR and a contact resistance that decreases with an increased temperature.

In order to better characterize ultra-thin W films, new wafers will have to be made. If these are made with W films with thicknesses around 1.6nm, the thickness at which the transition to continuous occurs can be characterized more precisely.

**Contents**

**Abstract** **iii**

**List of acronyms** **vii**

**1 Introduction** **1**

**2 Background** **3**

2.1 Conductivity in ultra-thin metal films . . . 3

2.2 CTLM structures . . . 4

2.3 Fabrication of test structures . . . 6

2.4 Measurement setup . . . 8

**3 Measurements** **9**
3.1 Visual inspection . . . 9

3.2 Sanity Checks . . . 10

3.2.1 Influence of the tests . . . 10

3.2.2 Uniformity of the wafer . . . 12

3.3 I/V measurements at room temperature . . . 13

3.3.1 Rt2 _{results . . . 18}

3.4 Temperature effects . . . 19

3.4.1 TCR Values . . . 19

3.4.2 Comparisons at various gap spacings and temperatures . . . . 22

**4 Conclusions and recommendations** **27**
4.1 Conclusions . . . 27

4.2 Recommendations . . . 27

**5 Acknowledgments** **29**

**References** **31**

**Appendices**

VI CONTENTS

**A Matlab scripts** **33**

**List of acronyms**

**W** tungsten

**CTLM** circular transfer length method

**HWALD** hot-wire assisted atomic layer deposition
**TCR** temperature coefficient of resistance

**Chapter 1**

**Introduction**

In integrated circuits ultra-thin conducting layers are used in a wide variety of appli-cations. Such ultra-thin layers behave differently from thick layers. One difference is that when such layers fall under a certain thickness, the so-called percolation threshold, the film will become discontinuous. This has a large effect on the film’s conductivity. As such it is important to know at which thickness the film becomes discontinuous. Another difference is that thick layers of metal have an increase in resistance when the temperature increases, but in thin layers that may be reversed. In this thesis measurements will be made on wafers on which ultra-thin layers of tungsten (W) have been grown by means of hot-wire assisted atomic layer deposition (HWALD). These wafers are of various thickness and have different test structures on them. Measurements will be made on circular transfer length method (CTLM) structures.

The goal of this thesis is to characterize electrical conductivity of ultra-thin W films. More specifically, the resistivity, voltage-dependent-resistance, contact resis-tance and temperature dependency of all those variables.

In chapter 2 the background for this assignment will be explained. That chapter will deal with conduction in ultra-thin films, a general explanation of CTLM structures, a more specific explanation of the structures used in this assignment and finally the measurement setup used. Chapter 3 deals with the measurement results. First up is the visual inspection, followed by sanity checks to find out if the measurements influence the W, followed by measurements at room temperature and finally mea-surements at temperatures ranging from 0 to 100 degrees centigrade. In chapter 4, conclusions are drawn and recommendations are made for further research.

**Chapter 2**

**Background**

**2.1**

**Conductivity in ultra-thin metal films**

If a metal film is extremely thin, it is discontinuous. In that case there are islands of the metal that are not interconnected. A current can still pass through the material, but the electrons will have to pass through a potential barrier. An externally applied voltage alters the height or shape of the barrier and as such the current does not scale linearly with the voltage.

If the metal film increases in thickness, the islands become larger and some of them become interconnected, resulting in a higher conductivity. If the metal layer keeps increasing in thickness, at a certain point all the metal will be connected and it has become continuous.

The thickness at which the transition between continuous and discontinuous
oc-curs is called the percolation threshold. Since discontinuities greatly reduce the
conductivity, it is important to know the value of this threshold for those applications
in which the metal is used as a conductor. The Rt2 _{method is one way to establish}

the value of the percolation threshold [1]. In that method, the resistance of the film times its thickness squared, is compared between the different film thicknesses. The threshold is at the thickness where this value is lowest.

**Temperature influence** Temperature dependency on resistivity is called the temperature
coefficient of resistance (TCR), indicated by parameter α[◦_{C}−1_{]. The equation for}

TCR is as follows:

ρ(T) =ρ(0)(1 +αT) (2.1)
Whereαis the TCR, T is the temperature in◦_{C and}_{ρ}_{(T) is the resistivity at a certain}

temperature. The equation can be rewritten as:

α=

ρ(T)

ρ(0) −1

T (2.2)

8 CHAPTER 2. BACKGROUND

All wafers have been made with the mask as shown in figure 2.4(a). In this thesis only the CTLM structure will be tested and they are shown in figures 2.4(b) and 2.4(c). The gap spacing between the inner and outer electrode varies between 2.5 and 300µm. In the A row of the CTLM matrix, the inner electrode has a diameter of 125µm. In the B and C rows that is 100 and 75µm respectively.

CTLM structure coordinates on the wafer are determined first by the number of the matrix it is in and then by the row and column within that matrix. For example, the top right CTLM structures are labeled 4A3.

The wafers were manufactured in mid 2016 and measured in late 2017 and early 2018.

**2.4**

**Measurement setup**

**Figure 2.5:** Measurement setup. On the left is a Temptronic temperature regulator.
In the center is a probe station with a microscope, probe needles and a
chuck with a wafer on it. On the right is a Keithley 4200 semiconductor
characterization system.

The measurement setup used for these experiments, is the Cascade setup at the University of Twente, which can be seen in figure 2.5. It consists of a microscope, four needles on which voltages and currents can be applied and measured and a temperature regulator.

In these tests two needles are used, one on the center electrode and one on the
big outside electrode, as can be seen in figure 2.1. The voltage applied between
those needles varies between -20 and +20 volt. To protect the wafers, the current is
limited to 100mA. The tests where temperature related phenomena are not tested,
are all performed at 25◦_{C. When those phenomena are tested, the temperature is}

**Chapter 3**

**Measurements**

**3.1**

**Visual inspection**

The first test I did was a visual inspection under the microscope. I noticed a lot of irregularities on the wafers, namely:

• Transparent circles of varying size that have rainbow colored edges.

• Gray circles of various size.

• Small black spots in various shapes.

• CTLM structures without a center electrode.

• CTLM structures where the center electrode was at least partially connected

to the outer electrode.

Figure 3.1 shows two of those irregularities. The circles in that figure show some similarity in appearance to condensation, but heating up the wafer did not get rid of them.

10 CHAPTER3. MEASUREMENTS

**Figure 3.1:** Image showing missing center electrodes and transparent
rainbow-color-edged circles.

Every wafer had some areas where no visual irregularities were observed. How-ever, the position of those areas varied from wafer to wafer, meaning that the mea-surements would not take place on the same position on each wafer.

**3.2**

**Sanity Checks**

**3.2.1**

**Influence of the tests**

3.2. SANITYCHECKS 11

**Figure 3.2:** Repeated I/V measurements of 2.5µm CTLM structure of 0.57nm thick
W

Figure 3.2 shows that the difference between those 4 measurements is not huge, but on that scale it is not possible to see if there is a small scale effect. Therefore in figure 3.3(a) the difference between the run from -20 to +20 volt and the run from +20 to -20 volt is plotted. There is a relatively large difference at low voltages, probably related to how the measurements are performed when crossing 0 volt. Other than that a systematic but very small (in the order of 0.1% of the total current) difference can be seen.

(a) Hysteresis per run (b) Difference between first and subsequent runs

**Figure 3.3:** Comparison between I/V measurements of 2.5µm CTLM structure of
0.57nm thick W

12 CHAPTER3. MEASUREMENTS

the order of 0.1% of the total current). This leads to the conclusion that testing does not alter the material in a significant manner.

**3.2.2**

**Uniformity of the wafer**

The results of the measurements should be independent of the position on the wafer. To test this, the same structure, in this case the CTLM structure with a 10µm gap and 0.57nm thickness, is tested at various locations on the wafer.

**Figure 3.4:** I/V characteristics of 0.57nm thick W measured on CTLM structures
with 10µm gap spacing at various places on the wafer.

Figure 3.4 shows the results of this test. Clearly there is no uniformity. The difference between the measurements on location 4a1 and 14a1 is about a factor 30. Though those are the locations that provide the extreme results, neither of them appears to be an outlier.

3.3. I/V MEASUREMENTS AT ROOM TEMPERATURE 13

**3.3**

**I/V measurements at room temperature**

While the sanity tests have shown that there is non-uniformity on the wafer, it is still possible that certain parameters, for instance transfer length, are the same regard-less of position. To test this, every I/V measurement has been performed on different positions on each wafer. Figure 3.5 shows one such measurement for every wafer.

14 CHAPTER3. MEASUREMENTS

(b) 0.9nm at position 6A1

3.3. I/V MEASUREMENTS AT ROOM TEMPERATURE 15

(d) 2.85nm at position 3A1

(e) 8.5nm at position 2A1

16 CHAPTER3. MEASUREMENTS

The expected result would be that as the film thickness increases, the I/V relation would become more linear and the conductivity would increase. However, the 1.6nm graph (3.5(c)) shows more linearity and conductivity than the 2.85nm graph (3.5(d)). A possible cause for that result is that at the tested location, the film at the waver that should have a W thickness of 1.6nm, is thicker than at the waver that should have a thickness of 2.85nm.

After applying the correction factor for CTLM measurements, the results are plot-ted in figure 3.6.

(a) 0.57nm:ρvalues of 0.184 and 0.730_{Ω}m (b) 0.9nm:ρvalues of 7.33 and 148mΩm

3.3. I/V MEASUREMENTS AT ROOM TEMPERATURE 17

(e) 8.5nm:ρvalues of 2.30 and 2.85µΩm

**Figure 3.6:** Resistance plotted against CTML gap spacing for W of various
thick-nesses. The correction factor as a result of the gap spacing has already
been applied.

In figure 3.6 the CTLM results of measurements on two positions of every film thickness are plotted. The squares are the measurement points and the solid lines are the linear regression of those measurements.

Thickness [nm] 0.57 0.9 1.6 2.85 8.5

Location Test 1 7A1 6A1 1A2 3A1 2A1

Location Test 2 12A2 3A1 19A2 19A1 8A1

Rc Test 1 [Ω] 1.13 x 106 1.95 x 104 14.1 46.8 10.3

Rc Test 2 [Ω] 4.01 x 106 1.13 x 106 71.0 17.6 10.5

LT Test 1 [µm] 1.48 1.02 9.09 2.78 13.1

LT Test 2 [µm] 1.33 2.91 10.2 6.26 16.4

R2_{* Test 1} _{0.987} _{0.994} _{0.983} _{0.990} _{0.995}

R2_{* Test 2} _{0.990} _{0.948} _{0.967} _{0.987} _{0.971}

Rsh Test 1 [Ω] 3.24 x 108 8.14 x 106 656 7.13 x 103 335

Rsh Test 2 [Ω] 1.28 x 109 1.65 x 108 2.96 x 103 1.19 x 103 271

ρTest 1 [Ωm] 0.184 7.33 x 10−3 _{1.05 x 10}−6 _{2.03 x 10}−5 _{2.85 x 10}−6

ρTest 2 [Ωm] 0.730 0.148 4.74 x 10−6 _{3.40 x 10}−6 _{2.30 x 10}−6

**Table 3.1:** Parameters derived from the plots in figure 3.6

*R2 _{is the regression coefficient}

18 CHAPTER3. MEASUREMENTS

instance on the 0.9nm thick measurements at location 3A1 with gap spacing 30 and 40 µm). This shows that there is a difference even between W layers that are positionally very close to each other.

As all the parameters depend on a linear regression of measurements where the only difference is the gap spacing and the previous paragraph shows that there are other differences, none of the parameters are reliable.

**3.3.1**

**Rt**

2 **results**

(a) 2.5µm gap (b) 5µm gap

**Figure 3.7:**

(a) 10µm gap (b) 20µm gap

**Figure 3.7:** Rt2 _{results for different gap spacings}

3.4. TEMPERATURE EFFECTS 19

cases the lowest Rt2_{is obtained at a film thickness of 1.6nm. Since the lowest value}

of that parameter is the thickness where the material goes from semi-continuous to continuous, according to this data this should occur around 1.6nm.

**3.4**

**Temperature effects**

**3.4.1**

**TCR Values**

20 CHAPTER3. MEASUREMENTS

(b) 0.9nm

3.4. TEMPERATURE EFFECTS 21

(d) 2.85nm

(e) 8.5nm

22 CHAPTER3. MEASUREMENTS

Figure 3.8 shows the TCR values of W at various thicknesses and voltages. All those measurements were taken at CTLM structures with a gap spacing of 10 µm. With the exception of the 8.5nm thick W films, all the TCR’s are negative, indicating that a higher temperature leads to a lower resistivity. There are two factors that play a role in the 8.5nm positive TCR. First, it is the thickest film being measured, so it will most closely resemble the thick-film behavior, which has a positive TCR. Second, that film has the lowest resistance (in the order of 20Ω), meaning that the contact resistance of the probes to the electrodes plays a big part. This can change between the different tests, as the needles may not be applied with the same pressure. It can be shown that this plays a factor by the big difference in the TCR values between the different values.

The TCR values of 1.6nm at 75◦_{C and 2.85nm at 100}◦_{C vary significantly from}

the other values at their respective thicknesses. This might also be due to different probe contact resistances.

The TCR value is voltage dependent, with the biggest voltage dependency shown at the 1.6nm thickness. In films up to 1.6nm in thickness, a lower voltage causes a higher absolute value of the TCR.

**3.4.2**

**Comparisons at various gap spacings and temperatures**

(a) 0.57nm at 1A2: αbetween -5.74 and -8.97
m◦_{C}−1

3.4. TEMPERATURE EFFECTS 23

(c) 1.6nm at 19A3: αbetween 0.312 and 0.810
m◦_{C}−1

(d) 2.85nm at 1A2: α between -1.01 and -1.11
m◦_{C}−1

(e) 8.5nm at 19A3: αbetween -1.98 and +0.196
m◦_{C}−1

**Figure 3.9:** Comparisons of W resistance at various thicknesses and temperatures

In figure 3.9, as in figure 3.5, the squares show the measurements and the solid lines the linear regression of those measurements.

Temperature[◦_{C]} _{0} _{25} _{50} _{75} _{100}

LT [µm] 7.92 7.77 6.60 6.55 6.26

Rc[Ω] 2.37 x 107 1.80 x 107 1.29 x 107 1.02 x 107 7.99 x 106

R2_{*} _{0.773} _{0.780} _{0.808} _{0.823} _{0.833}

Rsh [Ω] 1.27 x 109 9.84 x 108 8.31 x 108 6.60 x 108 5.41 x 108

ρ[Ωm] 0.724 0.561 0.474 0.376 0.309

α[◦_{C}−1_{]} _{-} _{-8.97 x 10}−3 _{-6.90 x 10}−3 _{-6.40 x 10}−3 _{-5.74 x 10}−3

24 CHAPTER3. MEASUREMENTS

Temperature[◦_{C]} _{0} _{25} _{50} _{75} _{100}

LT [µm] 13.6 13.4 12.4 11.7 11.0

Rc[Ω] 1.58 x 107 1.22 x 107 9.46 x 106 7.56 x 106 6.10 x 106

R2_{*} _{0.671} _{0.670} _{0.719} _{0.733} _{0.752}

Rsh [Ω] 4.93 x 108 3.88 x 108 3.24 x 108 2.74 x 108 2.35 x 108

ρ[Ωm] 0.444 0.349 0.291 0.247 0.212

α[◦_{C}−1_{]} _{-} _{-8.51 x 10}−3 _{-6.88 x 10}−3 _{-5.93 x 10}−3 _{-5.23 x 10}−3

**Table 3.3:** Result from measurements of 0.9nm thick W at location 2a1 as plotted in
3.9(b)

Temperature[◦_{C]} _{0} _{25} _{50} _{75} _{100}

LT [µm] 10.0 9.61 9.19 8.26 7.59

Rc[Ω] 59.0 57.1 54.9 51.2 48.3

R2_{*} _{0.983} _{0.984} _{0.988} _{0.992} _{0.993}

Rsh [Ω] 2.50 x 103 2.52 x 103 2.54 x 103 2.63 x 103 2.70 x 103

ρ[Ωm] 3.99 x 10−6 _{4.03 x 10}−6 _{4.06 x 10}−6 _{4.21 x 10}−6 _{4.32 x 10}−6

α[◦_{C}−1_{]} _{-} _{3.72 x 10}−4 _{3.12 x 10}−4 _{7.09 x 10}−4 _{8.10 x 10}−4

**Table 3.4:** Result from measurements of 1.6nm thick W at location 19a3 as plotted
in 3.9(c)

Temperature[◦_{C]} _{0} _{25} _{50} _{75} _{100}

LT [µm] 5.43 5.37 5.23 5.22 5.50

Rc[Ω] 115 110 105 102 104

R2_{*} _{0.919} _{0.921} _{0.924} _{0.926} _{0.924}

Rsh [Ω] 8.96 x 103 8.71 x 103 8.50 x 103 8.27 x 103 8.02 x 103

ρ[Ωm] 2.55 x 10−5 _{2.48 x 10}−5 _{2.42 x 10}−5 _{2.36 x 10}−5 _{2.28 x 10}−5

α[◦_{C}−1_{]} _{-} _{-1.11 x 10}−3 _{-1.01 x 10}−3 _{-1.02 x 10}−3 _{-1.05 x 10}−3

3.4. TEMPERATURE EFFECTS 25

Temperature[◦_{C]} _{0} _{25} _{50} _{75} _{100}

LT [µm] 12.0 13.0 14.0 10.6 10.9

Rc[Ω] 8.31 8.54 8.70 7.46 7.58

R2_{*} _{0.983} _{0.995} _{0.993} _{0.988} _{9.84}

Rsh [Ω] 293 279 264 298 295

ρ[Ωm] 2.49 x 10−6 _{2.37 x 10}−6 _{2.25 x 10}−6 _{2.53 x 10}−6 _{2.51 x 10}−6

α[◦_{C}−1_{]} _{-} _{-1.92 x 10}−3 _{-1.98 x 10}−3 _{1.96 x 10}−4 _{5.59 x 10}−5

**Table 3.6:** Result from measurements of 8.5nm thick W at location 19a3 as plotted
in 3.9(e)

*R2 _{is the regression coefficient}

**Chapter 4**

**Conclusions and recommendations**

**4.1**

**Conclusions**

There is a lot of difference between the W at various positions on the wafers. It is un-known if this is due to differences in thickness and/or impurities that have persisted since they were manufactured, or if it is due to non-homogeneous aging. As such, the other conclusions are tentative.

W films transfer from semi-continuous to continuous at a thickness of approxi-mately 1.6nm.

W films of a thickness up to at least 0.9nm, have a highly non-linear I/V relation-ship.

W films of a thickness up to at least 0.9nm, have a negative TCR.

W films of a thickness up to at least 0.9nm, have a voltage dependent TCR, with lower voltages providing a higher absolute value of TCR.

W films of a thickness up to at least 0.9nm, have a contact resistance that de-creases with an increased temperature.

**4.2**

**Recommendations**

To evaluate if HWALD produces a homogeneous W film, new wafers should be made. Shortly after production, measurements should take place on different loca-tions and both the results and localoca-tions should be documented.

Those wafers should be made at various thicknesses around 1.6nm, so that the percolation threshold can be determined with greater accuracy.

To evaluate the aging process of W films, the measurements should be repeated at set intervals. If previous measurements found that the W films were not homo-geneous, the measurements should be repeated at the same locations. If they are homogeneous, it is preferable to measure at different locations, as the measurement

28 CHAPTER 4. CONCLUSIONS AND RECOMMENDATIONS

**Chapter 5**

**Acknowledgments**

I would like to thank F.J. van der Velden and Mengdi Yang for designing and making the wafers respectively.

I would like to thank Satadal Duta for introducing me to the probe station and reserving time at it for me.

I would like to thank Alexey Kovalgin for supervising me during the thesis.

**Bibliography**

[1] I. Rycroft and B. Evans, “The in situ characterization of metal film resistance during deposition,” Thin Solid Films, vol. 290-291, pp. 283 – 288, 1996, papers presented at the 23rd International Conference on Metallurgical Coatings and Thin Films. [Online]. Available: http://www.sciencedirect.com/science/article/pii/ S004060909609181X

[2] D. C. Giancoli, “Physics for scientists & engineers with modern physics,” p. 762, 2014.

[3] K. Ren, F. Rao, Z. Song, S. Lv, M. Zhu, L. Wu, B. Liu, and S. Feng, “Study on the impact of the initialization process on the phase change memory,” vol. 102, 05 2013.

[4] J. H. Klootwijk and C. E. Timmering, “Merits and limitations of circular tlm struc-tures for contact resistance determination for novel iii-v hbts,” in Proceedings of the 2004 International Conference on Microelectronic Test Structures (IEEE Cat. No.04CH37516), March 2004, pp. 247–252.

[5] F. van der Velde, “Electrical measurement method and test structures for de-termining continuity of ultra-thin conducting or insulating films.” Master’s thesis, University of Twente, 2016.

[6] A. Y. Kovalgin, M. Yang, S. Banerjee, R. O. Apaydin, A. A. I. Aarnink, S. Kinge, and R. A. M. Wolters, “Hot-wire assisted ALD: A study powered by in situ spec-troscopic ellipsometry,” Advanced Material Interfaces, vol. 4, 2017.

[7] H. V. Bui, F. B. Wiggers, M. P. de Jong, and A. Y. Kovalgin, “An approach to characterize ultra-thin conducting films protected against native oxidation by an in-situ capping layer,” in 2014 International Conference on Microelectronic Test Structures (ICMTS), March 2014, pp. 53–57.

**Appendix A**

**Matlab scripts**

**A.1**

**I/V characteristics**

Matlab script that was used to generate figure 3.6 and parameters in table 3.1. In this case the values of the 0.57nm tests have been entered.

clear all clf

x=[50,40,30,20,10,5,2.5]; %gap spacicings in um t = 0.57; %thickness in nm

rad=62.5; %Radius of inner electrode in um

cor=rad./x .* log((rad+x)/rad); %correction factor for CTLM %resistances y1=[2.87E+07,2.58E+07,2.28E+07,1.68E+07,9.31E+06,5.32E+06,2.49E+06]; z1=[1.15E+08,9.94E+07,8.86E+07,6.49E+07,3.75E+07,1.91E+07,1.02E+07]; y2=y1./cor; z2=z1./cor; hold on;

p=polyfit(x,y2,1); %generates straight line q=polyfit(x,z2,1); x2=[-max([p(2)/p(1) q(2)/q(1)]),50]; y3=polyval(p,x2); z3=polyval(q,x2); plot(x2,y3,’red’); plot(x2,z3,’blue’); plot(x,y2,’s’,’MarkerEdgeColor’,’red’); plot(x,z2,’s’,’MarkerEdgeColor’,’blue’); ax = gca;

ax.YAxisLocation = ’origin’;

34 APPENDIX A. MATLAB SCRIPTS xlabel(’gap spacing[\mum]’); ylabel(’Resistance[\Omega]’); legend(’7a1’,’12a2’,’location’,’north’); title([num2str(t),’nm’]); xlim([x2(1) inf]); ylim([0 max(y3(2),z3(2))]); y4=polyval(p,x); z4=polyval(q,x);

Rsq1= 1 - sum((y2 - y4).^2)/sum((y2 - mean(y2)).^2);%regression coefficient Rsq2= 1 - sum((z2 - z4).^2)/sum((z2 - mean(z2)).^2);

Rsh1 = p(1)*(2*pi*rad); %sheet resistance Rsh2 = q(1)*(2*pi*rad);

rho1 = Rsh1 * t * 10^-9; %resistivity rho2 = Rsh2 * t * 10^-9;

Rc1 = p(2)/2; Rc2 = q(2)/2; Lt1 = p(2)/p(1)/2; Lt2 = q(2)/q(1)/2;

**A.2**

**Temperature dependencies**

Matlab script that was used to generate figure 3.9 and parameters in tables 3.2 through 3.6. In this case the values of the 0.57nm tests have been entered.

clear all clf

x=[50,40,30,20,10,5,2.5]; %gap spacicings in um t = 0.57; %thickness in nm

rad=62.5; %Radius of inner electrode in um

A.2. TEMPERATURE DEPENDENCIES 35 b4=a4./cor; b5=a5./cor; hold on; plot(x,b5,’s’,’MarkerEdgeColor’,’red’); plot(x,b4,’s’,’MarkerEdgeColor’,’green’); plot(x,b3,’s’,’MarkerEdgeColor’,’blue’); plot(x,b2,’s’,’MarkerEdgeColor’,’cyan’); plot(x,b1,’s’,’MarkerEdgeColor’,’magenta’); c1=polyfit(x,b1,1); %generates straight line c2=polyfit(x,b2,1);

c3=polyfit(x,b3,1); c4=polyfit(x,b4,1); c5=polyfit(x,b5,1);

d=[-max([c1(2)/c1(1) c2(2)/c2(1) c3(2)/c3(1) c4(2)/c4(1) c5(2)/c5(1)]),50]; e1=polyval(c1,d); e2=polyval(c2,d); e3=polyval(c3,d); e4=polyval(c4,d); e5=polyval(c5,d); plot(d,e5,’red’); plot(d,e4,’green’); plot(d,e3,’blue’); plot(d,e2,’cyan’); plot(d,e1,’magenta’); ax = gca;

ax.YAxisLocation = ’origin’; xlabel(’gap spacing[\mum]’); ylabel(’Resistance[\Omega]’);

legend(’0C’,’25C’,’50C’,’75C’,’100C’,’location’,’northwest’); title([num2str(t),’nm’]);

ylim([0 max([e1(2) e2(2) e3(2) e4(2) e5(2)])]); xlim([d(1) inf]); f1=polyval(c1,x); f2=polyval(c2,x); f3=polyval(c3,x); f4=polyval(c4,x); f5=polyval(c5,x);

36 APPENDIX A. MATLAB SCRIPTS

Rsq3= 1 - sum((b3 - f3).^2)/sum((b3 - mean(b3)).^2); Rsq4= 1 - sum((b4 - f4).^2)/sum((b4 - mean(b4)).^2); Rsq5= 1 - sum((b5 - f5).^2)/sum((b5 - mean(b5)).^2); Rsh1 = c1(1)*(2*pi*rad); %sheet resistance

Rsh2 = c2(1)*(2*pi*rad); Rsh3 = c3(1)*(2*pi*rad); Rsh4 = c4(1)*(2*pi*rad); Rsh5 = c5(1)*(2*pi*rad);

rho1 = Rsh1 * t * 10^-9; %resistivity rho2 = Rsh2 * t * 10^-9;

rho3 = Rsh3 * t * 10^-9; rho4 = Rsh4 * t * 10^-9; rho5 = Rsh5 * t * 10^-9; alpha4 = (rho4/rho5-1)/25; alpha3 = (rho3/rho5-1)/50; alpha2 = (rho2/rho5-1)/75; alpha1 = (rho1/rho5-1)/100; Rc1 = c1(2)/2;

Rc2 = c2(2)/2; Rc3 = c3(2)/2; Rc4 = c4(2)/2; Rc5 = c5(2)/2;